#------------------------------------------------------------------------------
#$Date: 2020-09-04 01:26:16 +0300 (Fri, 04 Sep 2020) $
#$Revision: 255834 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/36/4003665.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003665
loop_
_publ_author_name
'Shi, Shuangshuang'
'Lin, Chensheng'
'Yang, Guangsai'
'Cao, Liling'
'Li, Bingxuan'
'Yan, Tao'
'Luo, Min'
'Ye, Ning'
_publ_section_title
;
 A2Bi2(SeO3)3F2 (A = K and Rb): Excellent Mid-Infrared Nonlinear Optical
 Materials with Both Strong SHG Responses and Large Band Gaps
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.0c02837
_journal_year                    2020
_chemical_formula_sum            'Bi2 F2 O9 Rb2 Se3'
_chemical_formula_weight         1007.78
_space_group_IT_number           8
_space_group_name_Hall           'C -2y'
_space_group_name_H-M_alt        'C 1 m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 92.877(12)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.096(10)
_cell_length_b                   5.955(4)
_cell_length_c                   7.727(6)
_cell_measurement_reflns_used    1095
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4237
_cell_measurement_theta_min      3.1150
_cell_volume                     601.8(8)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type
;
Saturn724+ (2x2 bin mode)
;
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0430
_diffrn_reflns_av_sigmaI/netI    0.0773
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            2570
_diffrn_reflns_theta_full        27.45
_diffrn_reflns_theta_max         27.45
_diffrn_reflns_theta_min         3.11
_exptl_absorpt_coefficient_mu    46.369
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5975
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Colourless
_exptl_crystal_density_diffrn    5.562
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Brick
_exptl_crystal_F_000             864
_exptl_crystal_size_max          0.0500
_exptl_crystal_size_mid          0.0500
_exptl_crystal_size_min          0.0500
_refine_diff_density_max         1.694
_refine_diff_density_min         -1.855
_refine_diff_density_rms         0.341
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00
_refine_ls_extinction_coef       0.0064(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_reflns         1380
_refine_ls_number_restraints     20
_refine_ls_restrained_S_all      1.019
_refine_ls_R_factor_all          0.0354
_refine_ls_R_factor_gt           0.0328
_refine_ls_shift/su_max          0.008
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0092P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0605
_refine_ls_wR_factor_ref         0.0617
_reflns_number_gt                1314
_reflns_number_total             1380
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm0c02837_si_003.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_symmetry_cell_setting' value 'Monoclinic' was changed to
'monoclinic' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_cell_volume        601.8(7)
_cod_original_sg_symbol_H-M      'Cm   '
_cod_database_code               4003665
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x, -y, z'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.12098(5) 0.0000 0.46371(8) 0.0115(2) Uani 1 2 d S . .
Bi2 Bi 0.52696(5) 0.0000 -0.18907(6) 0.0102(2) Uani 1 2 d S . .
Rb1 Rb 0.3140(2) -0.5000 0.6472(3) 0.0161(5) Uani 1 2 d S . .
Se1 Se 0.39470(14) 0.0000 0.4248(2) 0.0106(4) Uani 1 2 d S . .
Se2 Se -0.07203(15) 0.0000 0.0960(2) 0.0103(4) Uani 1 2 d S . .
Rb2 Rb 0.23788(14) 0.0000 -0.0117(2) 0.0159(5) Uani 1 2 d S . .
Se3 Se 0.62585(14) 0.0000 0.2397(2) 0.0101(4) Uani 1 2 d S . .
O1 O 0.6991(7) 0.2151(16) 0.3212(11) 0.011(2) Uani 1 1 d U . .
F1 F 0.6388(6) -0.2442(13) 0.7232(11) 0.0176(18) Uani 1 1 d . . .
O2 O 0.4675(7) 0.2154(17) 0.5051(13) 0.027(3) Uani 1 1 d . . .
O3 O 0.0478(10) 0.0000 0.1795(16) 0.028(4) Uani 1 2 d S . .
O4 O -0.0712(7) -0.2217(17) -0.0384(13) 0.023(3) Uani 1 1 d U . .
O5 O 0.2975(9) 0.0000 0.5653(15) 0.012(3) Uani 1 2 d SU . .
O6 O 0.6542(9) 0.0000 0.0285(15) 0.013(3) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Bi1 O1 95.5(5) 3_445 4_455 ?
O1 Bi1 O3 73.9(3) 3_445 . ?
O1 Bi1 O3 73.9(3) 4_455 . ?
O1 Bi1 O5 73.2(3) 3_445 . ?
O1 Bi1 O5 73.2(3) 4_455 . ?
O3 Bi1 O5 130.2(4) . . ?
O1 Bi1 F1 143.5(3) 3_445 3_455 ?
O1 Bi1 F1 84.8(3) 4_455 3_455 ?
O3 Bi1 F1 139.5(2) . 3_455 ?
O5 Bi1 F1 72.0(3) . 3_455 ?
O1 Bi1 F1 84.8(3) 3_445 4_445 ?
O1 Bi1 F1 143.5(3) 4_455 4_445 ?
O3 Bi1 F1 139.5(2) . 4_445 ?
O5 Bi1 F1 72.0(3) . 4_445 ?
F1 Bi1 F1 74.4(4) 3_455 4_445 ?
O1 Bi1 O2 86.8(3) 3_445 3_445 ?
O1 Bi1 O2 152.6(3) 4_455 3_445 ?
O3 Bi1 O2 80.6(3) . 3_445 ?
O5 Bi1 O2 132.9(3) . 3_445 ?
F1 Bi1 O2 109.3(3) 3_455 3_445 ?
F1 Bi1 O2 63.9(3) 4_445 3_445 ?
O1 Bi1 O2 152.6(3) 3_445 4_455 ?
O1 Bi1 O2 86.8(3) 4_455 4_455 ?
O3 Bi1 O2 80.6(3) . 4_455 ?
O5 Bi1 O2 132.9(3) . 4_455 ?
F1 Bi1 O2 63.9(3) 3_455 4_455 ?
F1 Bi1 O2 109.3(3) 4_445 4_455 ?
O2 Bi1 O2 79.1(4) 3_445 4_455 ?
O1 Bi1 Rb2 50.7(2) 3_445 . ?
O1 Bi1 Rb2 50.7(2) 4_455 . ?
O3 Bi1 Rb2 46.2(3) . . ?
O5 Bi1 Rb2 84.0(3) . . ?
F1 Bi1 Rb2 134.24(19) 3_455 . ?
F1 Bi1 Rb2 134.24(19) 4_445 . ?
O2 Bi1 Rb2 115.5(2) 3_445 . ?
O2 Bi1 Rb2 115.5(2) 4_455 . ?
O1 Bi1 Rb1 114.9(2) 3_445 1_565 ?
O1 Bi1 Rb1 49.3(2) 4_455 1_565 ?
O3 Bi1 Rb1 122.45(18) . 1_565 ?
O5 Bi1 Rb1 47.38(6) . 1_565 ?
F1 Bi1 Rb1 42.00(19) 3_455 1_565 ?
F1 Bi1 Rb1 97.61(18) 4_445 1_565 ?
O2 Bi1 Rb1 151.0(2) 3_445 1_565 ?
O2 Bi1 Rb1 87.3(2) 4_455 1_565 ?
Rb2 Bi1 Rb1 93.38(6) . 1_565 ?
O1 Bi1 Rb1 49.3(2) 3_445 . ?
O1 Bi1 Rb1 114.9(2) 4_455 . ?
O3 Bi1 Rb1 122.45(18) . . ?
O5 Bi1 Rb1 47.38(6) . . ?
F1 Bi1 Rb1 97.61(18) 3_455 . ?
F1 Bi1 Rb1 42.00(19) 4_445 . ?
O2 Bi1 Rb1 87.3(2) 3_445 . ?
O2 Bi1 Rb1 151.0(2) 4_455 . ?
Rb2 Bi1 Rb1 93.38(6) . . ?
Rb1 Bi1 Rb1 92.80(8) 1_565 . ?
O1 Bi1 Rb2 108.0(2) 3_445 1_556 ?
O1 Bi1 Rb2 108.0(2) 4_455 1_556 ?
O3 Bi1 Rb2 177.0(3) . 1_556 ?
O5 Bi1 Rb2 52.8(3) . 1_556 ?
F1 Bi1 Rb2 39.49(18) 3_455 1_556 ?
F1 Bi1 Rb2 39.49(18) 4_445 1_556 ?
O2 Bi1 Rb2 97.1(2) 3_445 1_556 ?
O2 Bi1 Rb2 97.1(2) 4_455 1_556 ?
Rb2 Bi1 Rb2 136.78(7) . 1_556 ?
Rb1 Bi1 Rb2 59.11(4) 1_565 1_556 ?
Rb1 Bi1 Rb2 59.11(4) . 1_556 ?
F1 Bi2 F1 83.0(4) 2_554 1_554 ?
F1 Bi2 O6 75.9(3) 2_554 . ?
F1 Bi2 O6 75.9(3) 1_554 . ?
F1 Bi2 O4 167.7(3) 2_554 4_545 ?
F1 Bi2 O4 94.2(3) 1_554 4_545 ?
O6 Bi2 O4 91.8(3) . 4_545 ?
F1 Bi2 O4 94.2(3) 2_554 3 ?
F1 Bi2 O4 167.7(3) 1_554 3 ?
O6 Bi2 O4 91.8(3) . 3 ?
O4 Bi2 O4 86.0(5) 4_545 3 ?
F1 Bi2 Rb1 41.8(2) 2_554 3_554 ?
F1 Bi2 Rb1 41.8(2) 1_554 3_554 ?
O6 Bi2 Rb1 65.0(3) . 3_554 ?
O4 Bi2 Rb1 132.5(2) 4_545 3_554 ?
O4 Bi2 Rb1 132.5(2) 3 3_554 ?
F1 Bi2 Rb2 138.3(2) 2_554 . ?
F1 Bi2 Rb2 138.3(2) 1_554 . ?
O6 Bi2 Rb2 113.8(3) . . ?
O4 Bi2 Rb2 47.1(2) 4_545 . ?
O4 Bi2 Rb2 47.1(2) 3 . ?
Rb1 Bi2 Rb2 178.75(5) 3_554 . ?
F1 Bi2 Rb1 144.5(2) 2_554 1_554 ?
F1 Bi2 Rb1 83.2(2) 1_554 1_554 ?
O6 Bi2 Rb1 131.25(11) . 1_554 ?
O4 Bi2 Rb1 46.1(2) 4_545 1_554 ?
O4 Bi2 Rb1 105.5(2) 3 1_554 ?
Rb1 Bi2 Rb1 121.21(6) 3_554 1_554 ?
Rb2 Bi2 Rb1 59.51(5) . 1_554 ?
F1 Bi2 Rb1 83.2(2) 2_554 1_564 ?
F1 Bi2 Rb1 144.5(2) 1_554 1_564 ?
O6 Bi2 Rb1 131.25(11) . 1_564 ?
O4 Bi2 Rb1 105.5(2) 4_545 1_564 ?
O4 Bi2 Rb1 46.1(2) 3 1_564 ?
Rb1 Bi2 Rb1 121.21(6) 3_554 1_564 ?
Rb2 Bi2 Rb1 59.51(5) . 1_564 ?
Rb1 Bi2 Rb1 89.49(7) 1_554 1_564 ?
F1 Bi2 Rb2 37.0(2) 2_554 3 ?
F1 Bi2 Rb2 97.5(2) 1_554 3 ?
O6 Bi2 Rb2 47.91(10) . 3 ?
O4 Bi2 Rb2 132.5(2) 4_545 3 ?
O4 Bi2 Rb2 73.6(2) 3 3 ?
Rb1 Bi2 Rb2 59.89(5) 3_554 3 ?
Rb2 Bi2 Rb2 119.37(5) . 3 ?
Rb1 Bi2 Rb2 178.52(5) 1_554 3 ?
Rb1 Bi2 Rb2 90.65(6) 1_564 3 ?
F1 Bi2 Rb2 97.5(2) 2_554 3_545 ?
F1 Bi2 Rb2 37.0(2) 1_554 3_545 ?
O6 Bi2 Rb2 47.91(10) . 3_545 ?
O4 Bi2 Rb2 73.6(2) 4_545 3_545 ?
O4 Bi2 Rb2 132.5(2) 3 3_545 ?
Rb1 Bi2 Rb2 59.89(5) 3_554 3_545 ?
Rb2 Bi2 Rb2 119.37(5) . 3_545 ?
Rb1 Bi2 Rb2 90.65(6) 1_554 3_545 ?
Rb1 Bi2 Rb2 178.52(5) 1_564 3_545 ?
Rb2 Bi2 Rb2 89.17(6) 3 3_545 ?
F1 Rb1 F1 62.5(3) 3_445 4_445 ?
F1 Rb1 O2 167.6(3) 3_445 2 ?
F1 Rb1 O2 111.6(3) 4_445 2 ?
F1 Rb1 O2 111.6(3) 3_445 1_545 ?
F1 Rb1 O2 167.6(3) 4_445 1_545 ?
O2 Rb1 O2 71.9(4) 2 1_545 ?
F1 Rb1 O5 59.1(3) 3_445 1_545 ?
F1 Rb1 O5 120.0(3) 4_445 1_545 ?
O2 Rb1 O5 122.5(3) 2 1_545 ?
O2 Rb1 O5 52.5(3) 1_545 1_545 ?
F1 Rb1 O5 120.0(3) 3_445 . ?
F1 Rb1 O5 59.1(3) 4_445 . ?
O2 Rb1 O5 52.5(3) 2 . ?
O2 Rb1 O5 122.5(3) 1_545 . ?
O5 Rb1 O5 155.1(4) 1_545 . ?
F1 Rb1 O4 115.4(3) 3_445 4_546 ?
F1 Rb1 O4 89.1(3) 4_445 4_546 ?
O2 Rb1 O4 74.2(3) 2 4_546 ?
O2 Rb1 O4 103.2(3) 1_545 4_546 ?
O5 Rb1 O4 127.4(3) 1_545 4_546 ?
O5 Rb1 O4 76.8(3) . 4_546 ?
F1 Rb1 O4 89.1(3) 3_445 3_546 ?
F1 Rb1 O4 115.4(3) 4_445 3_546 ?
O2 Rb1 O4 103.2(3) 2 3_546 ?
O2 Rb1 O4 74.2(3) 1_545 3_546 ?
O5 Rb1 O4 76.8(3) 1_545 3_546 ?
O5 Rb1 O4 127.4(3) . 3_546 ?
O4 Rb1 O4 50.6(4) 4_546 3_546 ?
F1 Rb1 O1 65.9(2) 3_445 4_445 ?
F1 Rb1 O1 90.9(2) 4_445 4_445 ?
O2 Rb1 O1 104.4(3) 2 4_445 ?
O2 Rb1 O1 76.7(3) 1_545 4_445 ?
O5 Rb1 O1 53.8(3) 1_545 4_445 ?
O5 Rb1 O1 101.9(3) . 4_445 ?
O4 Rb1 O1 178.5(3) 4_546 4_445 ?
O4 Rb1 O1 130.6(2) 3_546 4_445 ?
F1 Rb1 O1 90.9(2) 3_445 3_445 ?
F1 Rb1 O1 65.9(2) 4_445 3_445 ?
O2 Rb1 O1 76.7(3) 2 3_445 ?
O2 Rb1 O1 104.4(3) 1_545 3_445 ?
O5 Rb1 O1 101.9(3) 1_545 3_445 ?
O5 Rb1 O1 53.8(3) . 3_445 ?
O4 Rb1 O1 130.6(2) 4_546 3_445 ?
O4 Rb1 O1 178.5(3) 3_546 3_445 ?
O1 Rb1 O1 48.1(3) 4_445 3_445 ?
F1 Rb1 Se1 86.23(17) 3_445 1_545 ?
F1 Rb1 Se1 141.94(18) 4_445 1_545 ?
O2 Rb1 Se1 94.4(2) 2 1_545 ?
O2 Rb1 Se1 27.37(17) 1_545 1_545 ?
O5 Rb1 Se1 28.1(2) 1_545 1_545 ?
O5 Rb1 Se1 136.3(2) . 1_545 ?
O4 Rb1 Se1 125.6(2) 4_546 1_545 ?
O4 Rb1 Se1 83.1(2) 3_546 1_545 ?
O1 Rb1 Se1 54.82(17) 4_445 1_545 ?
O1 Rb1 Se1 95.41(19) 3_445 1_545 ?
F1 Rb1 Se1 141.94(18) 3_445 . ?
F1 Rb1 Se1 86.23(17) 4_445 . ?
O2 Rb1 Se1 27.37(17) 2 . ?
O2 Rb1 Se1 94.4(2) 1_545 . ?
O5 Rb1 Se1 136.3(2) 1_545 . ?
O5 Rb1 Se1 28.1(2) . . ?
O4 Rb1 Se1 83.1(2) 4_546 . ?
O4 Rb1 Se1 125.6(2) 3_546 . ?
O1 Rb1 Se1 95.41(19) 4_445 . ?
O1 Rb1 Se1 54.82(17) 3_445 . ?
Se1 Rb1 Se1 110.58(10) 1_545 . ?
O2 Se1 O2 98.2(7) . 2 ?
O2 Se1 O5 100.9(4) . . ?
O2 Se1 O5 100.9(4) 2 . ?
O2 Se1 Rb1 51.5(3) . 1_565 ?
O2 Se1 Rb1 128.3(4) 2 1_565 ?
O5 Se1 Rb1 57.02(9) . 1_565 ?
O2 Se1 Rb1 128.3(4) . . ?
O2 Se1 Rb1 51.5(3) 2 . ?
O5 Se1 Rb1 57.02(9) . . ?
Rb1 Se1 Rb1 110.58(10) 1_565 . ?
O2 Se1 Rb2 125.7(4) . . ?
O2 Se1 Rb2 125.7(4) 2 . ?
O5 Se1 Rb2 100.0(4) . . ?
Rb1 Se1 Rb2 105.04(7) 1_565 . ?
Rb1 Se1 Rb2 105.04(7) . . ?
O3 Se2 O4 101.8(4) . . ?
O3 Se2 O4 101.8(4) . 2 ?
O4 Se2 O4 103.6(7) . 2 ?
O3 Se2 Rb1 133.6(5) . 3_454 ?
O4 Se2 Rb1 55.7(3) . 3_454 ?
O4 Se2 Rb1 55.7(3) 2 3_454 ?
O3 Se2 Rb2 130.84(5) . 3_445 ?
O4 Se2 Rb2 45.6(4) . 3_445 ?
O4 Se2 Rb2 119.1(3) 2 3_445 ?
Rb1 Se2 Rb2 65.30(4) 3_454 3_445 ?
O3 Se2 Rb2 130.84(5) . 3_455 ?
O4 Se2 Rb2 119.1(3) . 3_455 ?
O4 Se2 Rb2 45.6(4) 2 3_455 ?
Rb1 Se2 Rb2 65.30(4) 3_454 3_455 ?
Rb2 Se2 Rb2 98.07(8) 3_445 3_455 ?
F1 Rb2 F1 65.5(3) 4_444 3_454 ?
F1 Rb2 O3 89.7(3) 4_444 . ?
F1 Rb2 O3 89.7(3) 3_454 . ?
F1 Rb2 O4 126.9(3) 4_444 3 ?
F1 Rb2 O4 90.4(3) 3_454 3 ?
O3 Rb2 O4 139.1(2) . 3 ?
F1 Rb2 O4 90.4(3) 4_444 4_545 ?
F1 Rb2 O4 126.9(3) 3_454 4_545 ?
O3 Rb2 O4 139.1(2) . 4_545 ?
O4 Rb2 O4 66.7(4) 3 4_545 ?
F1 Rb2 O1 143.1(2) 4_444 4_455 ?
F1 Rb2 O1 102.5(2) 3_454 4_455 ?
O3 Rb2 O1 54.3(2) . 4_455 ?
O4 Rb2 O1 85.9(2) 3 4_455 ?
O4 Rb2 O1 121.4(3) 4_545 4_455 ?
F1 Rb2 O1 102.5(2) 4_444 3_445 ?
F1 Rb2 O1 143.1(2) 3_454 3_445 ?
O3 Rb2 O1 54.3(2) . 3_445 ?
O4 Rb2 O1 121.4(3) 3 3_445 ?
O4 Rb2 O1 85.9(2) 4_545 3_445 ?
O1 Rb2 O1 65.3(3) 4_455 3_445 ?
F1 Rb2 O6 54.5(3) 4_444 3_445 ?
F1 Rb2 O6 115.3(3) 3_454 3_445 ?
O3 Rb2 O6 69.5(2) . 3_445 ?
O4 Rb2 O6 144.0(3) 3 3_445 ?
O4 Rb2 O6 77.5(3) 4_545 3_445 ?
O1 Rb2 O6 110.7(3) 4_455 3_445 ?
O1 Rb2 O6 49.2(3) 3_445 3_445 ?
F1 Rb2 O6 115.3(3) 4_444 3_455 ?
F1 Rb2 O6 54.5(3) 3_454 3_455 ?
O3 Rb2 O6 69.5(2) . 3_455 ?
O4 Rb2 O6 77.5(3) 3 3_455 ?
O4 Rb2 O6 144.0(3) 4_545 3_455 ?
O1 Rb2 O6 49.2(3) 4_455 3_455 ?
O1 Rb2 O6 110.7(3) 3_445 3_455 ?
O6 Rb2 O6 137.7(4) 3_445 3_455 ?
F1 Rb2 O5 54.6(2) 4_444 1_554 ?
F1 Rb2 O5 54.6(2) 3_454 1_554 ?
O3 Rb2 O5 136.1(3) . 1_554 ?
O4 Rb2 O5 72.7(2) 3 1_554 ?
O4 Rb2 O5 72.7(2) 4_545 1_554 ?
O1 Rb2 O5 147.28(17) 4_455 1_554 ?
O1 Rb2 O5 147.28(17) 3_445 1_554 ?
O6 Rb2 O5 101.0(2) 3_445 1_554 ?
O6 Rb2 O5 101.0(2) 3_455 1_554 ?
F1 Rb2 Se1 147.24(16) 4_444 . ?
F1 Rb2 Se1 147.24(16) 3_454 . ?
O3 Rb2 Se1 89.3(2) . . ?
O4 Rb2 Se1 69.7(2) 3 . ?
O4 Rb2 Se1 69.7(2) 4_545 . ?
O1 Rb2 Se1 52.10(16) 4_455 . ?
O1 Rb2 Se1 52.10(16) 3_445 . ?
O6 Rb2 Se1 94.9(2) 3_445 . ?
O6 Rb2 Se1 94.9(2) 3_455 . ?
O5 Rb2 Se1 134.6(2) 1_554 . ?
F1 Rb2 Se3 127.35(18) 4_444 3_455 ?
F1 Rb2 Se3 77.13(18) 3_454 3_455 ?
O3 Rb2 Se3 53.24(8) . 3_455 ?
O4 Rb2 Se3 87.0(2) 3 3_455 ?
O4 Rb2 Se3 142.3(2) 4_545 3_455 ?
O1 Rb2 Se3 25.35(15) 4_455 3_455 ?
O1 Rb2 Se3 85.63(18) 3_445 3_455 ?
O6 Rb2 Se3 121.8(2) 3_445 3_455 ?
O6 Rb2 Se3 25.3(2) 3_455 3_455 ?
O5 Rb2 Se3 126.30(7) 1_554 3_455 ?
Se1 Rb2 Se3 76.15(6) . 3_455 ?
O6 Se3 O1 102.1(4) . . ?
O6 Se3 O1 102.1(4) . 2 ?
O1 Se3 O1 97.6(6) . 2 ?
O6 Se3 Rb2 53.88(13) . 3_545 ?
O1 Se3 Rb2 122.8(3) . 3_545 ?
O1 Se3 Rb2 52.3(3) 2 3_545 ?
O6 Se3 Rb2 53.88(13) . 3 ?
O1 Se3 Rb2 52.3(3) . 3 ?
O1 Se3 Rb2 122.8(3) 2 3 ?
Rb2 Se3 Rb2 100.13(8) 3_545 3 ?
O6 Se3 Rb1 128.2(4) . 3 ?
O1 Se3 Rb1 51.7(3) . 3 ?
O1 Se3 Rb1 51.7(3) 2 3 ?
Rb2 Se3 Rb1 99.48(6) 3_545 3 ?
Rb2 Se3 Rb1 99.48(6) 3 3 ?
Se3 O1 Bi1 118.6(4) . 3 ?
Se3 O1 Rb1 103.2(4) . 3 ?
Bi1 O1 Rb1 97.1(3) 3 3 ?
Se3 O1 Rb2 102.4(4) . 3 ?
Bi1 O1 Rb2 95.0(3) 3 3 ?
Rb1 O1 Rb2 141.8(3) 3 3 ?
Bi2 F1 Bi1 127.5(3) 1_556 3_545 ?
Bi2 F1 Rb1 106.7(3) 1_556 3 ?
Bi1 F1 Rb1 101.0(3) 3_545 3 ?
Bi2 F1 Rb2 115.1(3) 1_556 3_546 ?
Bi1 F1 Rb2 105.8(3) 3_545 3_546 ?
Rb1 F1 Rb2 94.7(2) 3 3_546 ?
Se1 O2 Bi1 148.4(6) . 3 ?
Se1 O2 Rb1 101.2(4) . 1_565 ?
Bi1 O2 Rb1 102.5(3) 3 1_565 ?
Se2 O3 Bi1 133.9(8) . . ?
Se2 O3 Rb2 127.3(6) . . ?
Bi1 O3 Rb2 98.8(4) . . ?
Se2 O4 Bi2 148.5(5) . 3_445 ?
Se2 O4 Rb2 111.0(5) . 3_445 ?
Bi2 O4 Rb2 96.8(3) 3_445 3_445 ?
Se2 O4 Rb1 97.6(4) . 3_454 ?
Bi2 O4 Rb1 99.4(3) 3_445 3_454 ?
Rb2 O4 Rb1 85.2(2) 3_445 3_454 ?
Se1 O5 Bi1 121.7(6) . . ?
Se1 O5 Rb1 94.8(2) . 1_565 ?
Bi1 O5 Rb1 97.2(2) . 1_565 ?
Se1 O5 Rb1 94.8(2) . . ?
Bi1 O5 Rb1 97.2(2) . . ?
Rb1 O5 Rb1 155.1(4) 1_565 . ?
Se1 O5 Rb2 145.4(5) . 1_556 ?
Bi1 O5 Rb2 92.9(4) . 1_556 ?
Rb1 O5 Rb2 79.5(2) 1_565 1_556 ?
Rb1 O5 Rb2 79.5(2) . 1_556 ?
Se3 O6 Bi2 121.1(6) . . ?
Se3 O6 Rb2 100.8(2) . 3 ?
Bi2 O6 Rb2 99.7(2) . 3 ?
Se3 O6 Rb2 100.8(2) . 3_545 ?
Bi2 O6 Rb2 99.7(2) . 3_545 ?
Rb2 O6 Rb2 137.7(4) 3 3_545 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O1 2.291(9) 3_445 ?
Bi1 O1 2.291(9) 4_455 ?
Bi1 O3 2.351(12) . ?
Bi1 O5 2.404(11) . ?
Bi1 F1 2.520(8) 3_455 ?
Bi1 F1 2.520(8) 4_445 ?
Bi1 O2 2.660(10) 3_445 ?
Bi1 O2 2.660(10) 4_455 ?
Bi1 Rb2 4.050(3) . ?
Bi1 Rb1 4.111(3) 1_565 ?
Bi1 Rb1 4.111(3) . ?
Bi1 Rb2 4.260(3) 1_556 ?
Bi2 F1 2.196(8) 2_554 ?
Bi2 F1 2.196(8) 1_554 ?
Bi2 O6 2.307(12) . ?
Bi2 O4 2.429(11) 4_545 ?
Bi2 O4 2.429(11) 3 ?
Bi2 Rb1 4.026(4) 3_554 ?
Bi2 Rb2 4.090(3) . ?
Bi2 Rb1 4.230(3) 1_554 ?
Bi2 Rb1 4.230(3) 1_564 ?
Bi2 Rb2 4.242(2) 3 ?
Bi2 Rb2 4.242(2) 3_545 ?
Rb1 F1 2.803(8) 3_445 ?
Rb1 F1 2.803(8) 4_445 ?
Rb1 O2 2.888(10) 2 ?
Rb1 O2 2.888(10) 1_545 ?
Rb1 O5 3.049(3) 1_545 ?
Rb1 O5 3.049(3) . ?
Rb1 O4 3.088(10) 4_546 ?
Rb1 O4 3.088(10) 3_546 ?
Rb1 O1 3.141(9) 4_445 ?
Rb1 O1 3.141(9) 3_445 ?
Rb1 Se1 3.622(3) 1_545 ?
Rb1 Se1 3.622(3) . ?
Se1 O2 1.697(9) . ?
Se1 O2 1.697(9) 2 ?
Se1 O5 1.714(12) . ?
Se1 Rb1 3.622(3) 1_565 ?
Se1 Rb2 3.860(3) . ?
Se2 O3 1.667(13) . ?
Se2 O4 1.680(10) . ?
Se2 O4 1.680(10) 2 ?
Se2 Rb1 3.706(4) 3_454 ?
Se2 Rb2 3.943(2) 3_445 ?
Se2 Rb2 3.943(2) 3_455 ?
Rb2 F1 2.816(8) 4_444 ?
Rb2 F1 2.816(8) 3_454 ?
Rb2 O3 2.957(14) . ?
Rb2 O4 3.015(10) 3 ?
Rb2 O4 3.015(10) 4_545 ?
Rb2 O1 3.144(9) 4_455 ?
Rb2 O1 3.144(9) 3_445 ?
Rb2 O6 3.193(5) 3_445 ?
Rb2 O6 3.193(5) 3_455 ?
Rb2 O5 3.398(12) 1_554 ?
Rb2 Se3 3.883(2) 3_455 ?
Se3 O6 1.692(12) . ?
Se3 O1 1.702(9) . ?
Se3 O1 1.702(9) 2 ?
Se3 Rb2 3.883(2) 3_545 ?
Se3 Rb2 3.883(2) 3 ?
Se3 Rb1 3.899(4) 3 ?
O1 Bi1 2.291(9) 3 ?
O1 Rb1 3.141(9) 3 ?
O1 Rb2 3.144(9) 3 ?
F1 Bi2 2.196(8) 1_556 ?
F1 Bi1 2.520(8) 3_545 ?
F1 Rb1 2.803(8) 3 ?
F1 Rb2 2.816(8) 3_546 ?
O2 Bi1 2.660(10) 3 ?
O2 Rb1 2.888(10) 1_565 ?
O4 Bi2 2.429(11) 3_445 ?
O4 Rb2 3.015(10) 3_445 ?
O4 Rb1 3.088(10) 3_454 ?
O5 Rb1 3.049(3) 1_565 ?
O5 Rb2 3.398(12) 1_556 ?
O6 Rb2 3.193(5) 3 ?
O6 Rb2 3.193(5) 3_545 ?
